Plastic Deformation of Single Nanometer-Sized knordlun/pub/ Plastic Deformation of Single
Embed Size (px)
Transcript of Plastic Deformation of Single Nanometer-Sized knordlun/pub/ Plastic Deformation of Single
Plastic Deformation of Single Nanometer-Sized Crystals
Litao Sun,1,2 Arkady V. Krasheninnikov,3,4 Tommy Ahlgren,3 Kai Nordlund,3 and Florian Banhart5,* 1Key Laboratory of MEMS of Ministry of Education, Southeast University, Nanjing 210096, China
2Institut für Physikalische Chemie, Universität Mainz, D-55099 Mainz, Germany 3Materials Physics Division, University of Helsinki, P.O. Box 43, FI-00014, Finland
4Laboratory of Physics, Helsinki University of Technology, P.O. Box 1100, FI-02015, Finland 5Institut de Physique et Chimie des Matériaux IPCMS-GSI, UMR 7504, 23 rue du Loess, 67034 Strasbourg, France
(Received 17 April 2008; published 7 October 2008)
We report in situ electron microscopy observations of the plastic deformation of individual nanometer-
sized Au, Pt, W, and Mo crystals. Specifically designed graphitic cages that contract under electron
irradiation are used as nanoscopic deformation cells. The correlation with atomistic simulations shows
that the observed slow plastic deformation is due to dislocation activity. Our results also provide evidence
that the vacancy concentration in a nanoscale system can be smaller than in the bulk material, an effect
which has not been studied experimentally before.
DOI: 10.1103/PhysRevLett.101.156101 PACS numbers: 61.72.Cc, 62.25.�g, 62.50.�p, 68.37.Og
Materials consisting of crystallites with sizes of a few nanometers have shown outstanding mechanical properties [1,2], for example, exceptionally high strength or hardness. Although such materials are already in use in industrial applications, their response to deformation and the mecha- nisms of inevitable creep at high temperature are still far from being understood. This is in part due to the deforma- tion behavior of such systems which is fundamentally different from that in their bulk counterparts [3,4]. Another reason is the lack of direct experimental informa- tion on defect dynamics in nanocrystalline materials. The field is dominated by atomistic simulations [5–8] which, although they have provided much insight, are limited to the nanosecond time scale.
Several experimental attempts have been undertaken to study the deformation mechanisms in various systems of submicron dimensions. Information about the response of nanosystems to stress was obtained by measuring the electrical conductance of nanowires under straining . In situ straining experiments on nanocrystalline bulk ma- terials have been done in an electron microscope , and the role of grain-boundary-mediated processes versus dis- location activity was discussed. Experiments  on thin films and patterned lines also indicate that the early stage plasticity is strongly size-dependent. Thus, information on the plastic deformation of isolated nanometer-sized crys- tals may be crucial for understanding the deformation mechanisms in nanocrystalline materials, but it has not been studied experimentally to date.
Here we report experiments that allow the slow defor- mation of single nanocrystallites with simultaneous obser- vation at the atomic scale by in situ high-resolution transmission electron microscopy (TEM). Metal crystals were exposed to pressure in graphitic nanocontainers that were designed for deformation experiments by electron beam structuring.
The principle of the experiment is shown schematically in Fig. 1. Graphitic nanocontainers are used as extrusion cells [12,13]. Au, Pt, Mo, and W crystals of a few nano- meters in size were encapsulated inside graphitic shells by coevaporation in an arc discharge  and irradiated with electrons (300 keV) in a temperature range of 300–1000 �C in the heating stage of a TEM. Under electron irradiation in a wide beam, the particles
became spherical due to surface stress which is exerted by the graphitic shells upon the removal of atoms and recon- struction [15,16]. Then the electron beamwas focused onto a spot of 2 nm in diameter and directed onto a point at the projected circumference of the graphitic shells. After 10– 20 seconds, the puncturing caused a hole  (2–3 nm in diameter) through which the material under pressure could escape. Then the beam was spread again over the whole particle. During the continuing collapse of the shells [12,14,17], pressure was built up, and the solid metal was gradually extruded through the hole. Because of the slow contraction of graphitic shells, the deformation occurs on a
FIG. 1 (color). Mechanism of the experiment: Graphitic shells encapsulating a metal crystal (a) are punctured by a focused electron beam (b). Successive electron irradiation of the carbon container leads to the contraction of the shells and extrusion of the metal crystal (c). The red circles indicate the diameter of the electron beam.
PRL 101, 156101 (2008) P HY S I CA L R EV I EW LE T T E R S week ending
10 OCTOBER 2008
0031-9007=08=101(15)=156101(4) 156101-1 � 2008 The American Physical Society
scale of 0:1–1 nm=s. This allows us to study the stability of nanocrystals in detail under continuous load.
Figure 2 shows the gradual extrusion of a Au crystal from a graphitic shell (’’carbon onion’’) at 300 �C. The puncturing of the shells was carried out between images (a) and (b). Grain boundaries appear repeatedly at the bottle- neck in the Au crystal where the deformation rate is the highest. In other encapsulated Au crystals, twins were occasionally observed at 300 �C and below.
In the bulk regions of the crystals, both inside and out- side, no visible defects appear. The faceting of the free Au surfaces outside the shells is apparent. The same experi- ment with Au at 600 �C is shown in Fig. 3. The process (a)– (f) happened within 12 minutes. No crystallographic de- fects appear, even in the bottleneck.
The same experiment with Pt (TEM images are shown in the supplementary material ) at 380 �C shows the formation of planar defects spreading over the whole crys- tal inside the shell. During the extrusion, stacking faults and twin boundaries appear, aligned in the direction of shear (through the hole). At 600 �C, the same behavior as for Au at 300 �C is seen (grain boundaries at the bottle- neck, but no defects in the bulk). Further experiments were carried out with Pt up to 900 �C, showing qualitatively the same behavior as Au at 600 �C. The extrusion of Pt crystals is slower than for Au at the same temperature and under the same irradiation conditions.
The extrusion of Mo or W crystals (both in the fcc phase) turned out to be impossible within the temperature
range of these experiments (
diffusion which can be associated with Herring-Nabarro creep; (2) diffusion of metal atoms at the metal-carbon interface (similar to Coble creep); and (3) plastic deforma- tion due to the nucleation and glide of dislocations or the creation of planar defects.
High pressure in the nonextruded part of the metal particles indicates that the self-diffusivity (mechanism 1) or surface diffusivity (mechanism 2) must be slow; other- wise, no pressure buildup inside the opened shells would be possible. To check this conjecture, we calculated the material transfer due to self-diffusion at different tempera- tures and pressures; see  for details of calculations. We have assumed a vacancy concentration as in thermal equi- librium and that the vacancy formation energy Ef in the
extruded part of the particle is the same as in the bulk system. We have taken the geometry of the experiment and assumed that diffusion is governed by vacancy migration. Hence, the vacancy flux is strongly influenced by a pres- sure gradient. Surprisingly, we found that the diffusion should be fast enough to provide efficient mass transfer for Au already at 300 �C and for Pt at 600 �C, which is inconsistent with the observation of considerable pressure (15–25 GPa) inside the cells.
An explanation of this pretended contradiction is that Ef in small crystals is higher than in the bulk, so that vacancy concentration and, correspondingly, self-diffusivity are low. This is a controversial issue: It has been previously suggested  that Ef should decrease with system size, as
cohesive energy and melting temperature of a small parti- cle drop. However, recent simulations  and our esti- mates  indicate that Ef can be larger for small particles
than in the bulk systems. Our experimental results are consistent with a higher value of Ef for small particles
and provide experimental evidence that the equilibrium vacancy concentration in small particles is indeed smaller than in bulk metals.
Similar arguments can be used to explain why mass transfer due to adatom diffusion (at the interface between metal and carbon) is suppressed. The separation between the graphitic shell and the metal in the uncompressed case is quite small (2–2.7 Å) . Thus, it costs more energy (0.5–1 eV or more depending on pressure ) to place a metal atom into the space between the compressing graph- itic shell and the metal than on a free metal surface, so it requires more than 3 eV to create an adatom-vacancy pair. Hence the carbon atom concentration at the metal-graphite interface should be negligible.
In order to explore the deformation by the nucleation and motion of dislocations, we carried out molecular dy- namics computer simulations . We concentrated on Pt as the typical fcc metal. The effect of contracting carbon shells on metal particles with typical diameters of about 4– 8 nm (as in experiments) was modeled by an external repulsive potential mimicking the shrinking carbon shells.
Figures 4(a)–4(c) show